DOI: 10.15632/jtam-pl.55.4.1341

**AN ANALYTICAL APPROACH TO PREDICTION OF INTERNAL DEFECTS**
**DURING THE FLAT ROLLING PROCESS OF STRAIN-HARDENING**

**MATERIALS**

Parvaneh Amjadian, Heshmatollah Haghighat

*Razi University, Mechanical Engineering Department, Kermanshah, Iran*
*e-mail: hhaghighat@razi.ac.ir*

In this paper, the upper bound method has been used in analysis of the flat rolling process and prediction of internal defects for a strain-hardening material. The arc of contact has been replaced by a chord. The inlet shear boundary of the deformation zone has been assumed as an exponential curve and the boundary at the exit has been assumed as a cylindrical surface. A kinematically admissible velocity field has been proposed and internal, shear and frictional power terms have been derived. By minimizing the total power with respect to the neutral point position and the shape of the inlet shear boundary, the rolling torque has been determined. A criterion has been presented to predict the occurrence of the internal defects for given rolling conditions. Comparison of the analytically developed approach for rolling torque and internal defects with published theoretical and experimental data shows generally good agreement.

*Keywords:*upper bound, flat rolling, internal defects, strain-hardening exponent

**1.** **Introduction**

Flat rolling is the process of reducing thickness of a long sheet by torques applied through a set of
rolls. The rolling process widely is used in production of industrial components, so concentrating
on the final quality of the parts produced by this process is very important. Internal central
bursts are common rolling processing defects. Ignoring their prediction causes both losses of
physical injury and property damage or reducing quality of the final products. Usually, it is
very difficult to detect central bursting defects by surface inspection. The investigations on
flat rolling have been conducted for decades and various aspects of these processes have been
studied. Dyja and Pietrzyk (1983) analyzed an asymmetric dual hot-rolled sheet using minimum
*energy, and replaced the arc of contact by a chord. Avitzur et al. (1988) modeled the flat*
rolling process by using upper bound analysis for rigid perfectly plastic materials to predict
*internal defects. Takuda et al. (1989) analyzed the strip rolling process by assuming a simple*
velocity field by considering free deformation zones in front and behind the roll gap. Turczyn
and Pietrzyk (1992) analyzed the effect of deformation zone geometry on the internal defect
in the flat rolling process. They used the upper bound method and took into consideration
velocity boundaries. Discontinuity circular arcs were present and uniform velocity fields for
internal defects assumed. Prakash and Dixit (1995) proposed a model for steady state plane
strain cold rolling of a strain-hardening material which could predict the roll force and torque
with reasonable engineering accuracy over the usual range of process variables. Turczyn (1996)
analyzed the effect of deformation zone geometry on the internal defects in rolling process using
the upper bound method. Martins and Barata (1999) presented an approach for analyzing plane
strain rolling. They used the upper bound method to estimate the rolling torque and to model the
material flow within the region of deformation between the rolls. Dogruoglu (2001) introduced a

systematic method for constructing kinematically admissible velocity fields, which was necessary
in the analysis of the plastic forming process by the upper bound method. Gosh and Gardiner
(2004) identified various modeling issues that were necessary for successful simulation of the cold
rolling process by comparing it with experiments on aluminum alloys. Rajak and Reddy (2005)
analyzed internal defects in the plane strain rolling process with the finite element method. They
used critical damage criteria. Serajzadeh and Mahmoodkhani (2008) presented a combined upper
bound and finite element model for prediction of velocity and temperature fields during the hot
rolling process. The closing behavior of internal defects in the central part of a continuous casting
steel slab during rough transverse rolling was investigated by using FE-code, ANSYS/LS-DYNA
*by Deng et al. (2009). Misicko et al. (2009) observed and analyzed by computer simulation*
behavior of artificial surface defects inside flat steel samples during the hot rolling process by
*selected parameters. Cao et al. (2015) investigated the prediction of damage for the ultimate*
wire flat rolling process of high carbon steel using three different approaches of ductile damage.
Haghighat and Saadati (2015) presented the kinematically admissible velocity field for the rolling
of sandwich sheets, non-bonded before rolling, and discussed some mathematical aspects by
the upper bound method. Haghighat and Pargzadeh (2017) investigated the effect of strain
hardening on the central bursting defects in rod extrusion process. In this paper, analyses of
plastic deformation and prediction of internal defects in flat rolling process of a strain-hardening
material using the upper bound method is considered. The arc of contact between the roll and
the sheet is replaced by a chord. Based on the FEM, it is observed that the inlet and outlet
shear boundaries are not circular and in any condition such as inlet thickness and reduction in
area are deferent, then we present arbitrary exponential shear boundaries and velocity field that
can predict rolling torque and internal defects. Then a kinematically admissible velocity field is
proposed and internal, shear and frictional power terms are derived. By minimizing the total
power with respect to the neutral point position and the shape of the inlet shear boundary, the
rolling torque and the occurrence of internal defects is investigated. The effect of the friction
factor, strain-hardening exponent and reduction in the area on the rolling torque and safe and
unsafe domains are investigated.

**2.** **Upper bound analysis**

Figure 1 shows flat rolling process parameters in a schematic diagram. Because of symmetry of
the process, only half of the section is considered. An important subject in the upper bound
analysis is the assumption of shear boundaries and a kinematically admissible velocity field
satis-fying volume constancy in the deformation zone and boundary conditions. In order to determine
the velocity field, the arc of contact is replaced by a chord. The material starts as a sheet of
*thickness ti* *and then is deformed into a sheet of thickness 2tf, vi* is the initial velocity of the

*sheet and vf* *is the velocity of the product, α is the angle of the line connecting the initial point*

*to the final point of the contact arc with the axis of symmetry. R is radius, and ω is angular*
velocity of the roll.

**2.1.** **Velocity zones**

To analyze the process, the material under deformation is divided into three deformation
*zones, as shown in Fig. 1. In zones I and III, the material moves rigidly with the velocity vi*

*and vf*, respectively. Zone II is the deformation zone and is surrounded by two shear surfaces

*S*1 *and S*2 *and the contact surface S*3*. The shear boundary S*2 at the exit from the deformation
*zone is assumed to be a cylindrical surface with its center at the apex O. The shear boundary S*1

Fig. 1. Geometry of the sheet, roll, deformation zone and the shear boundaries

is assumed to be an arbitrarily curved surface. Using this description, mathematical equations
*of the shear boundaries S1* *and S2* are defined in the cylindrical coordinates by

*ri(θ, ρi) = ρi*exp

h*b(θ − α)*
*α*

i

*rf(θ, ρf) = ρf* (2.1)

*where ri* *and rf* are the radial position of inlet and outlet shear boundary, respectively, and the

radial position in the deformation zone is
*r(θ, ρ) = ρ exp*h*b(θ − α)*
*α*
*ρ − ρf*
*ρi− ρf*
i
*= ρg(θ, ρ)* (2.2)

*where ρiand ρf* are the radial distances from the virtual apex to inlet and outlet shear boundaries

*on the roll surface shown in Fig. 1, b is the shape factor of the shear boundary at the inlet of*
*deformation zone II, θ is the peripheral position and ρ is the radial position on the contact*
*surface, and g is an arbitrary shape function*

*g(θ, ρ) = exp*h*b(θ − α)*
*α*
*ρ − ρf*
*ρi− ρf*
i
(2.3)
*b can be negative, zero or positive. When b is negative, the shear boundary moves away from the*
*origin O, when b is positive the shear boundary moves towards the apex O, when b is zero, the*
*inlet shear boundary is a cylindrical surface (i.e. g = 1). In zone I and III, the material moves*
*as a rigid body in the axial direction. In zone III, the velocity vf* from the volume flow balance

is

*vf* *= vi*

*ρi*

*ρf*

(2.4) With regard to the equilibrium of volume flow, the admissible velocity filed in deformation zone II can be obtained as

*vx(dy) = − ˙Ur(rdθ)* (2.5)

*vx* is the horizontal velocity component in the deformation zone, ˙*Ur* is the radial component of

*velocity and y is the vertical position.*

So, the radial velocity component of the velocity field is
˙
*Ur* *= −*
*vx*
*r*
*dy*
*dθ* *= −vi*
*ρi*
*ρ*
*cos θ +*1
*g*
*∂g*
*∂θ* *sin θ*
(2.6)
The volume constancy in the cylindrical coordinates system is defined as

*dotεrr+ ˙εθθ+ ˙εzz* = 0 (2.7)

According to the cylindrical coordinates strain rates components and the assumption of the
plane strain process, ˙*Uz* = 0 (lateral velocity component), the peripheral velocity component

( ˙*Uθ*) is
˙
*Uθ* *= viρi*
*∂g*
*∂rsin θ* (2.8)
where
*∂g*
*∂r* =
*∂g*
*∂ρ*
*∂ρ*
*∂r* =
*b(θ − α)*
*α*
1
*ρi− ρf*
1
1 +*b(θ−α) _{α}*

_{ρ}*ρ*

*i−ρf*(2.9)

The velocity components in deformation zone II are given as
˙
*Ur* *= −vi*
*ρi*
*ρ*
*cos θ +* 1
*g*
*∂g*
*∂θsin θ*
˙
*Uθ* *= viρi*
*∂g*
*∂rsin θ* *U*˙*z* = 0 (2.10)

As it is clear from Eqs. (2.10), on the axis of symmetry ˙*Uθ* = 0, and on the contact surface

between the roll and sheet ˙*Uθ*= 0, so the incompressibility condition is satisfied. Nonzero strain

rate components in the deformation zone are
*˙εrr= vi*
*ρi*
*ρ*2
1
*g*
h
*1 − ρ∂g*
*∂r*
*cos θ +*1
*g*
*∂g*
*∂θ* *− ρ*
*∂*2_{g}*∂r∂θ*
*sin θ*i
*˙εθθ* *= −vi*
*ρi*
*ρ*2
1
*g*
h
*1 − ρ∂g*
*∂r*
*cos θ +*1
*g*
*∂g*
*∂θ* *− ρ*
*∂*2_{g}*∂r∂θ*
*sin θ*i
*˙εrθ*=
1
2*vi*
*ρi*
*ρ*2
1
*g*
nh
*ρ*2*∂*
2_{g}*∂r*2 +
1
*g*2
*∂g*
*∂θ*
2
*−*1* _{g}∂*
2

_{g}*∂θ*2 + 1 i

*sin θ +*1

*g*

*∂g*

*∂θcos θ*o (2.11)

**2.2.** **Determinations of power terms**

The internal power in the upper bound analysis for a perfectly elasic von Mises material in the deformation zone is

˙
*Wi* = *√*2
3*σ0*
Z
*V*
r
1
2*˙εij˙εij* *dV* (2.12)

where ˙*Wi* *is internal power of deformation, σ*0 *is the average flow stress and dV is a differential*
volume of the deformation zone.

After substitution and simplification, the internal power of region II is given by
˙
*Wi* =
*2σ*0
*√*
3
*α*
Z
0
*ρi*
Z
*ρf*
q
*˙ε*2
*rr+ ˙ε*2*rθρg*
*g + ρ∂g*
*∂ρ*
*dρ dθ* (2.13)

The shear power loss at the shear boundary is
˙
*WS*=
*σ0*
*√*
3
Z
*S*1*,S*2
*|∆v| dS* (2.14)

where ˙*WS* *is the shear power loss along the shear boundary, ∆v is the velocity difference and*

each surface of velocity discontinuity, the area of discontinuity and the amount of velocity di-scontinuity must be determined. With attention to Fig. 1

*dS*1*= ρig(θ, ρi*)
s
1 +*b*
*α*
2
*dθ*
*|∆v*1*| =*
*vi*
*1 − ρi*
*∂g*
*∂r*
1
*1 + (b/α)*2
s
1 +*b*
*α*
*sin θ*
(2.15)

*thus the shear power loss on the shear surface S*1 is obtained as

˙
*WS*1 =
*σ*0
*√*
3*viρi*
h
1 +*b*
*α*
2i
*α*
Z
0
*g(θ, ρi*)
*1 − ρi*
*∂g*
*∂r*
1
*1 + (b/α)*2
*sin θ dθ* (2.16)

*also for the shear surface S*2, the differential area and the amount of velocity discontinuity can
be obtained respectively by

*dS2* *= ρfdθ* *|∆v*2*| = |vfsin θ|* (2.17)

*the shear power loss on the shear surface S*2 is obtained as

˙
*WS*2 =
*σ*0
*√*
3*vfρf*
*α*
Z
0
*sin θ dθ* (2.18)

*The friction power loss at the interface of the sheet and the roll in S3* and its general relation is
˙
*Wf* =
*mσ*0
*√*
3
Z
*S*3
*|∆v| dS* *dS*3*= dρ*
*∆v =*
*U*˙*r|θ=α+ Rω*
=
*− vi*
*ρi*
*ρ*
*cos α +* *b*
*α*
*ρ − ρf*
*ρi− ρf*
*sin α**+ Rω*
(2.19)

where ˙*Wf* *is the friction power loss, dS*3 *is a differential area of the frictional surface and m is*
the friction factor after simplification

˙
*Wf* *= m*
*σ0*
*√*
3*viρi*
*ρi*
Z
*ρf*
1
*ρ*
*cos α +*
*b*
*α*
*ρ − ρf*
*ρi− ρf* *sin α −*
*Rωρ*
*viρi*
*dρ* (2.20)

In the rolling process, there is only one point along the surface of contact between the roll and
the sheet at which the surface velocity of the roll equals to the velocity of the sheet. This point
is called the neutral point. Between the inlet shear surface and the neutral point the sheet is
moving slower than the roll surface and on the exit side of the neutral point, the sheet moves
faster than the roll surface. The position of the neutral point is where the relative velocity is
zero, then
*vi*
*ρi*
*ρN*
*cos α +* *b*
*α*
*ρN* *− ρf*
*ρi− ρf*
*sin α** _{− Rω = 0}* (2.21)

**2.3.** **Effective flow stress**

Since actual metals exhibit strain-hardening behavior and the upper bound method is based
on the assumption of perfectly elastic material, amendments must be made to match the
*the-oretical and actual behavior. For a plastic material, the mean flow stress of the material σ*0 is
given by
*σ*0=
1
*ε*
*ε*
Z
0
*σ dε* *ε =* *√*2
3ln
*ti*
*tf*
(2.22)
In this paper, a modified upper bound method is used and behavior of the material is considered
as

*σ = K(ε)n* (2.23)

*where K is the strength coefficient, n is the strain-hardening exponent, σ is the effective flow*
*stress and ε is effective strain. Inserting Eqs. (2.23) into Eq. (2.22), the mean flow stress of the*
material is given by
*σ*0=
1
*n + 1K*
2
*√*
3ln
*ti*
*tf*
*n*
(2.24)
According to Fig. 1, in all three zones each particle of the material undergoes different strains.
The material in zone I has no strain-hardening, at the inlet shear boundary it has a strain due
to discontinuity of velocity, in zone II the material undergoes strain due to deformation, after it,
at the outlet shear boundary the material undergoes strain due to discontinuity of velocity and,
finally, it exits from zone III with no deformation. By integrating the incremental strain along
*a stream line, the equivalent strain in the product is calculated. It has an angle of inclination θ*
*to the axis in the deformation zone. At the shear surface, the engineering shear strain γS* is

*γS*= *|∆v|*_{˙}

*Ur*

(2.25) and the effective strain on the shear boundary is

*εS* =

1
*√*

3*γS* (2.26)

At the inlet and outlet shear boundaries, the effective strains are, respectively

*εS*1 =
1
*√*
3*γS*1 =
1
*√*
3
*1 − ρi∂g _{∂r}_{1+(b/α)}*1 2
r
1 +

*2*

_{α}b*sin θ*

*cos θ +*1

_{g}∂g_{∂θ}sin θ*εS*2 = 1

*√*3

*γS*2 = 1

*√*3

*tan θ*(2.27)

In the deformation zone, the effective strain is expressed by
*εd*=
*ri*
Z
*rf*
*dε =*
*ri*
Z
*rf*
*dε*
*dt*
*dt*
*dL* *dL* (2.28)
where
*dε*
*dt* *= ˙ε =*
r
2
3*( ˙ε*
2
*rr+ ˙ε*2*θθ+ 2 ˙ε*2*rθ*) =
2
*√*
3
q
*˙ε*2
*rr+ ˙ε*2*rθ*
*dt*
*dL* =
1
q
˙
*U*2
*r* + ˙*Uθ*2
(2.29)

where
*dL = dr*
s
*1 + r*2*dθ*
*dr*
2
(2.30)
then
*εd*=
2
*√*
3
*ri*
Z
*rf*
v
u
u
t
*˙ε*2
*rr+ ˙ε*2*rθ*
˙
*U*2
*r* + ˙*Uθ*2
h
*1 + r*2*dθ*
*dr*
2i
*dr* (2.31)

Along the stream line, the equivalent strain in the deformed material is

*ε(θ) = εS*1*(θ) + εd(θ) + εS*2*(θ)* (2.32)

After obtaining the total strain from Eq. (2.32) and substituting in the power law, one can
rewrite the power terms in order to modify the upper bound method with considering the
*strain-hardening. So the internal power, shear loss powers on S*1 *and S*2 surfaces and the frictional
power, respectively, are

˙
*Wi* =
Z
*V*
*σ ˙ε dV =* *√*2
3
Z
*V*
*K(ε)n*
r
1
2*˙εij˙εij* *dV*
˙
*WS* =
Z
*Sv*
*τ |∆v| dS =* *√*1
3
Z
*V*
*K(ε)n _{|∆v| dS}*
˙

*Wf*= Z

*Sf*

*τ |∆v| dS =*

*√m*3 Z

*V*

*K(ε)n*(2.33)

_{|∆v| dS}**2.4.** **The required rolling torque**

By make use of the upper bound method, the externally supplied power is less than or equal
*to the sum of the powers described in the previous Sections. The total power J∗* _{is}

*J∗* _{= ˙}_{W}

*i*+ ˙*WS*1+ ˙*WS*2+ ˙*Wf* (2.34)

*The rolling torque T is given by*
*T =* *J∗*

*ω* (2.35)

*where T is the required rolling torque per unit width of the sheet. The rolling torque is a function*
*of b (shape factor) and ρN* *(position of the neutral point). The shape factor b determines the*

*inlet shear boundary shape. The minimum value of rolling torque with respect to b is the*
required torque for the rolling process in the upper bound analysis. Integrals appearing in the
above equations do not have analytical solutions and they have been solved numerically with
MATLAB software.

**3.** **Internal defects prediction criteria**

The external torque is a function of several parameters including roll radius, area reduction,
*friction factor and shape factor b. In the upper bound analysis, the minimum value of the*
*external power with respect to b is the required power for the rolling process. According to the*

Fig. 2. Geometrical condition to initiate the internal defect

*geometrical condition, for the critical value of shape factor b (bcr*), the inlet shear boundary

intersects the outlet shear boundary in the centerline, see Fig. 2. In this study, it can be taken that

*ri(θ = 0, ρi) = rf(θ = 0, ρf*) (3.1)

thus

*ρiexp(−b) = ρf* (3.2)

*so, the critical value of b can be obtained as*
*bcr* = ln
*ρi*
*ρf*
= ln *ti*
*tf*
(3.3)
So, if the shape parameter obtained from the optimization of the external power is equal or
*greater than the bcr*, the internal defects initiate.

**4.** **Results and discussion**

The flat rolling process has been analyzed using the proposed approach. In order to obtain
numerical boundaries that can be applied to the prediction and prevention of the occurrence of
internal defects in industry, finite element simulations using the proposed approach have been
carried out for many combinations of reduction in the area and relative thickness. This means
that no internal defects occur under this combination of process parameters. FEM simulations are
conducted on the available commercial explicit/FEM software, ABAQUS, to verify the analytical
model and study the effects of the upper bound method assumptions on the obtained results.
Due to symmetry of the process, finite element meshes are generated on the upper half cross
section of the sheet. The sheet is meshed by 2D plane strain, linear, four-noded CPE4R elements.
The sheet model contains 460 elements. In this model, the rolls are modeled as rigid bodies.
The rolls are rotated by a constant angular velocity about their axes. For verification of the
theoretical study, the results of rolling torque are extracted from FEM simulations. In order
to verify the validity of the upper bound approach for the flat rolling process presented in
the previous Sections, the results obtained from the theoretical model are compared with the
available experimental of data of Martins and Barata (1999) as well as with the results of finite
element simulations. The calculation has been carried out under various rolling conditions and
geometrical data utilized in the rolling analysis summarized in Table 1. During theoretical
*analysis and numerical simulations, m is set at 0.3 for the contact surface between the roll*
*and sheet, radius of the rolls is R = 79.375 mm, and the flow stress for aluminum at room*
*temperature is σ = 50.3(1 + ε/0.05)0.26*MPa. The comparisons between the computed results,

**Table 1.**Geometrical data used for computations (Martins and Barata, 1999)
Case *2t*0 *2tf* Reduction
[mm] [mm] [%]
1 6.274 5.385 14.17
2 6.274 4.902 21.86
3 6.274 4.445 29.40
4 6.274 4.115 34.41

Fig. 3. (a) Comparison of analytical, FEM and Martins experimental data (Martins and Barata, 1999) of rolling torque (per unit of width) as a function of the percentage of reduction. (b) Variation of rolling

*torque per unit width versus parameter b*

FEM simulation and the experimental values of Martins and Barata (1999) for the rolling torque
as a function of the rolling reduction are shown in Fig. 3a. It is observed that the proposed
velocity field leads to a computationally efficient procedure which gives a good agreement with
the experimental data. From Fig. 3a, it can be seen that the calculated torques are basically in
agreement with the measured ones. As expected, the predicted rolling torques are always greater
than the experimental and FEM results, because the present theoretical values are the upper
bound solutions. The reason for such discrepancies may be attributed to the assumption of rigid
rolls as well as to difficulties in the modeling of friction in the contact surface between the rolls
and the deforming sheet. It can be checked from Fig. 3a that the rolling torque increases with an
*increase in reduction. Figure 3b shows variation of the rolling load versus the shape parameter b*
for several reductions of the area according to Table 1. The internal defects criterion is achieved
after obtaining the shape parameter from both geometrical and analytical conditions and by
comparing them. In Fig. 4, the velocity components obtained from the upper bound solution are
*compared with the FEM simulation results in θ = α/2 in the deformation zone. The results show*
a good agreement between the upper bound data and the FEM results. It can be seen that the
peripheral velocity components are very small with respect to the radial velocity components.
To compare the numerical results with the experimental results of Ghos and Gardiner (2004),
the analysis performed on Aluminum 6061-T6 whose mechanical and physical properties are
shown in Table 2.

*The flow stress for aluminum at room temperature is σ = 410(ε)0.05*MPa (Turczyn, 1996).
*The initial thickness is ti* *= 10 mm, roll radius R = 100 mm, angular velocity ω = 0.167 s−1* and

*friction factor m = 0.3. Figure 5 shows the conditions of area reduction and relative thickness*
for preventing internal defects in Aluminum 6061-T6 for both conditions of strain-hardening

Fig. 4. Comparison of the upper bound and FEM of velocity components (a) radial and (b) peripheral velocity components for 30% reduction in the area

**Table 2.**Mechanical properties of Aluminum 6061-T6 (Turczyn, 1996)
Young’s Poisson’s Yield

Density [kg/m3]

Strength

Strain-modulus ratio stress coefficient -hardening

[GPa] *(ν)* [MPa] [MPa] exponent

68.9 0.33 276 2700 410 0.05

Fig. 5. Comparison of safe and unsafe zones predicted by the present model and the model by Turczyn (1996)

and perfectly plastic materials. Also, these results are compared with the experimental data by Turczyn (1996). It is observed that the safe domain is decreased by including the strain-hardening behavior of the material in the analysis.

*Figure 6a shows the velocity field in the flat rolling process with relative thickness 2ti/R = 0.2*

and 40% reduction in area. The velocity field shows that in this case the internal defects do not
occurr. In another model, see Fig. 6b, the reduction of the area is changed to 20% and the
*relative thickness is 2ti/R = 0.4, so that it locates in the unsafe zone. Also, Fig. 6b shows that*

*Fig. 6. Deformation zone, (a) for 2ti/R = 0.2 and 40% reduction in the area, (b) for 2ti/R = 0.4 and*

20% reduction in the area

Figure 8 shows the effect of friction factor on internal defects initiation situations for Alu-minum 6061-T6. It can be seen that with an increase in the friction factor, the safe zone size decreases. The effect of the strain-hardening exponent on the inlet shear boundary is shown in Fig. 8. From this figure, it can be noticed that with an increase in the strain-hardening exponent, the intersection point of the inlet shear boundary with the axis of symmetry moves towards the outside of the rolls, and the tendency of central bursting defects is decreased. Also, the criterion applied for different strain-hardening exponents is illustrated in Fig. 9a. This figure shows that with an increase in the strain-hardening exponent value, the safe domain increases. Figure 9b shows the effect of strain-hardening exponent on the rolling torque for the upper bound appro-ach and the FEM. This figure illustrates that by increasing the strain-hardening exponent, the rolling torque decreases. Figure 9b also shows that the theoretically predicted rolling torque is higher than that from the FEM results, which is due to the nature of the upper bound theory.

Fig. 7. Effect of the friction factor on size of the safe and unsafe zones

Fig. 9. Effect of the strain-hardening exponent (a) on size of the safe and unsafe zones and (b) on the rolling torque for 30% reduction in the area

**5.** **Conclusions**

In this paper, an analytical approach based on the upper bound method, is presented for predic-tion of rolling torque and occurrence of internal defects in the flat rolling process. The advantages of the presented criterion are the generality of the proposed inlet shear boundary and a new kinematically admissible velocity field. In addition, the presented criterion predicts central bur-sting defects in simpler mathematical equations than in other criteria, and the effect of the strain hardening exponent of the sheet material on the rolling torque and prediction of internal defects are investigated. It has been concluded that internal defects are affected primarily by the strain-hardening exponent. By increasing the strain-hardening exponent, the rolling torque and the possibility of internal defects decreases. By increasing the strain-hardening exponent, the safe zone size is increased and the internal defects occur in thick sheets with a small reduction. Criteria curves for the safe domains are presented for a wide range of process variables. By using these criteria in the rolling practice, it has become possible to predict necessary rolling conditions in order to avoid internal defects.

**References**

1. Avitzur B., Van Tyne C., Turczyn S., 1988, The prevention of central bursts during rolling,

*Journal of Engineering for Industry*, 110-173

2. Caoa T., Bobadillab C., Montmitonneta P., Bouchard P., 2015, A comparative study
*of three ductile damage approaches for fracture prediction in cold forming processes, Journal of*

*Materials Processing Technology***, 216, 385-404**

3. Deng W., Zhao D., Qin X., Du L., Gao X., Wang G., 2009, Simulation of central crack
* closing behavior during ultra-heavy plate rolling, Computational Materials Science, 47, 439-447*
4. Dogruoglu A., 2001, On constructing kinematically admissible velocity fields in cold sheet rolling,

*Journal of Materials Processing Technology***, 110, 287-299**

5. Dyja H., Pietrzyk M., 1983, On the theory of the process of hot rolling of bimetal plate and
**sheet, International Journal of Mechanical Working Technology, 8, 309-325**

6. Ghosh S., Li M., Gardiner D., 2004, A computational and experimental study of cold rolling
**of aluminum alloys with edge cracking, Transactions of the ASME, 126, 74-82**

7. Haghighat H., Amjadian P., 2013, A generalized upper bound solution for extrusion of
*bi-metallic rectangular cross-section bars through dies of any shape, Journal of Theoretical and Applied*

*Mechanics***, 51, 105-116**

8. Haghighat H., Parghazeh A., 2017, An investigation into the effect of strain hardening on the
*central bursting defects in rod extrusion process, The International Journal of Advanced *

*Manufac-turing Technology*, accepted for publication

9. Haghighat H., Saadati P., 2015, An upper bound analysis rolling process of non-bonded
**san-dwich sheets, Transaction of Nonferrous Metals Society of China, 25, 1605-1613**

10. Martins P., Barata M., 1999, Upper bound analysis of plane strain rolling using a flow function
*and the weighted residuals method, International Journal for Numerical Methods in Engineering,*

**44**, 1671-1683

11. Misicko R., Kvackaj T., Vlado M., Gulova L., Luptak M., Bidulska J., 2009, Defects
**simulation of rolling strips, Materials Engineering, 16, 7-12**

12. Prakash R., Dixit P., 1995, Steady state plane strain cold rolling of a strain-hardening material,

*Journal of Materials Processing Technology***, 52, 338-358**

*13. Rajak S., Reddy N., 2005, Prediction of internal defects in plane strain rolling, Journal of*

*Materials Processing Technology***, 159, 409-417**

14. Serajzadeh S., Mahmoodkhani Y., 2008, A combined upper bound and finite element model
*for prediction of velocity and temperature fields during hot rolling process, International Journal*

*of Mechanical Sciences***, 50, 1423-1431**

15. Takuda H., Kyoto H., Lippmann H., Kokado J., 1989, Upper bound approach to plane strain
**strip rolling with free deformation zones, Ingenieur-Archiv, 59, 274-284**

*16. Turczyn S., 1996, The effect of the roll-gap shape factor on internal defects in rolling, Journal of*

*Materials Processing Technology***, 60, 275-282**

17. Turczyn S., Pietrzyk M., 1992, The effect of deformation zone geometry on internal defects
**arising in plane strain rolling, Journal of Materials Processing Technology, 32, 509-518**